Colloidal Crystal Order and Structure Revealed by Tabletop Extreme Ultraviolet Scattering and Coherent Diffractive Imaging
Total Page：16
File Type：pdf, Size：1020Kb
Vol. 26, No. 9 | 30 Apr 2018 | OPTICS EXPRESS 11393 Colloidal crystal order and structure revealed by tabletop extreme ultraviolet scattering and coherent diffractive imaging 1,7,8 1,7,9 GIULIA F. MANCINI, ROBERT M. KARL JR., ELISABETH R. 1 1 1 SHANBLATT, CHARLES S. BEVIS, DENNIS F. GARDNER, MICHAEL D. 1 2,3 1 TANKSALVALA, JENNIFER L. RUSSELL, DANIEL E. ADAMS, HENRY C. 1 2,3,4,5 2,3,4,6 KAPTEYN, JOHN V. BADDING, THOMAS E. MALLOUK, AND 1 MARGARET M. MURNANE 1JILA, University of Colorado, 440 UCB, Boulder, CO 80309-0440, USA 2Department of Chemistry, Penn State University, University Park, PA 16802, USA 3Materials Research Institute, Penn State University, University Park, PA 16802, USA 4Department of Physics, Penn State University, University Park, PA 16802, USA 5Department of Materials Science and Engineering, Penn State University, University Park, PA 16802, USA 6Department of Biochemistry and Molecular Biology, Penn State University, University Park, PA 16802, USA 7These authors contributed equally to this work [email protected] [email protected] Abstract: Colloidal crystals with specific electronic, optical, magnetic, vibrational properties, can be rationally designed by controlling fundamental parameters such as chemical composition, scale, periodicity and lattice symmetry. In particular, silica nanospheres -which assemble to form colloidal crystals- are ideal for this purpose, because of the ability to infiltrate their templates with semiconductors or metals. However characterization of these crystals is often limited to techniques such as grazing incidence small-angle scattering that provide only global structural information and also often require synchrotron sources. Here we demonstrate small-angle Bragg scattering from nanostructured materials using a tabletop- scale setup based on high-harmonic generation, to reveal important information about the local order of nanosphere grains, separated by grain boundaries and discontinuities. We also apply full-field quantitative ptychographic imaging to visualize the extended structure of a silica close-packed nanosphere multilayer, with thickness information encoded in the phase. These combined techniques allow us to simultaneously characterize the silica nanospheres size, their symmetry and distribution within single colloidal crystal grains, the local arrangement of nearest-neighbor grains, as well as to quantitatively determine the number of layers within the sample. Key to this advance is the good match between the high harmonic wavelength used (13.5nm) and the high transmission, high scattering efficiency, and low sample damage of the silica colloidal crystal at this wavelength. As a result, the relevant distances in the sample - namely, the interparticle distance (≈124nm) and the colloidal grains local arrangement (≈1μm) – can be investigated with Bragg coherent EUV scatterometry and ptychographic imaging within the same experiment simply by tuning the EUV spot size at the sample plane (5μm and 15μm respectively). In addition, the high spatial coherence of high harmonics light, combined with advances in imaging techniques, makes it possible to image near-periodic structures quantitatively and nondestructively, and enables the observation of the extended order of quasi-periodic colloidal crystals, with a spatial resolution better than 20nm. In the future, by harnessing the high time-resolution of tabletop high harmonics, this technique can be extended to dynamically image the three-dimensional electronic, magnetic, and transport properties of functional nanosystems. © 2018 Optical Society of America under the terms of the OSA Open Access Publishing Agreement #321043 https://doi.org/10.1364/OE.26.011393 Journal © 2018 Received 6 Feb 2018; revised 28 Mar 2018; accepted 3 Apr 2018; published 18 Apr 2018 Vol. 26, No. 9 | 30 Apr 2018 | OPTICS EXPRESS 11394 OCIS codes: (340.7460) X-ray microscopy; (290.5820) Scattering measurements; (340.7480) X-rays, soft x-rays, extreme ultraviolet (EUV). References and links 1. J. L. Russell, G. H. Noel, J. M. Warren, N.-L. L. Tran, and T. E. Mallouk, “Binary Colloidal Crystal Films Grown by Vertical Evaporation of Silica Nanoparticle Suspensions,” Langmuir 33(39), 10366–10373 (2017). 2. T. Li, A. J. Senesi, and B. Lee, “Small Angle X-ray Scattering for Nanoparticle Research,” Chem. Rev. 116(18), 11128–11180 (2016). 3. J. E. Han and V. H. Crespi, “Tuning Fermi-surface properties through quantum confinement in metallic metalattices: new metals from old atoms,” Phys. Rev. Lett. 86(4), 696–699 (2001). 4. J. E. Han and V. H. Crespi, “Abrupt Topological Transitions in the Hysteresis Curves of Ferromagnetic Metalattices,” Phys. Rev. Lett. 89(19), 197203 (2002). 5. M. J. Kosterlitz and D. J. Thouless, “Ordering, metastability and phase transitions in two-dimensional systems,” J. Phys. Chem. 6, 1181–1203 (1973). 6. M. T. Barako, A. Sood, C. Zhang, J. Wang, T. Kodama, M. Asheghi, X. Zheng, P. V. Braun, and K. E. Goodson, “Quasi-ballistic Electronic Thermal Conduction in Metal Inverse Opals,” Nano Lett. 16(4), 2754–2761 (2016). 7. M. A. Boles, M. Engel, and D. V. Talapin, “Self-Assembly of Colloidal Nanocrystals: From Intricate Structures to Functional Materials,” Chem. Rev. 116(18), 11220–11289 (2016). 8. J. Miao, T. Ishikawa, I. K. Robinson, and M. M. Murnane, “Beyond crystallography: Diffractive imaging using coherent x-ray light sources,” Science 348(6234), 530–535 (2015). 9. M. Altarelli, R. P. Kurta, and I. A. Vartanyants, “X-ray cross-correlation analysis and local symmetries of disordered systems: General theory,” Phys. Rev. B 82, 104207 (2010). 10. R. P. Kurta, M. Altarelli, E. Weckert, and I. A. Vartanyants, “X-ray cross-correlation analysis applied to disordered two-dimensional systems,” Phys. Rev. B 85, 184204 (2012). 11. P. Wochner, C. Gutt, T. Autenrieth, T. Demmer, V. Bugaev, A. D. Ortiz, A. Duri, F. Zontone, G. Grübel, and H. Dosch, “X-ray cross correlation analysis uncovers hidden local symmetries in disordered matter,” Proc. Natl. Acad. Sci. U.S.A. 106(28), 11511–11514 (2009). 12. P. Wochner, M. Castro-colin, S. N. Bogle, and V. N. Bugaev, “Of fluctuations and cross-correlations: finding order in disorder,” Int. J. Mater. Res. 102, 874–888 (2011). 13. F. Lehmkühler, B. Fischer, L. Müller, B. Ruta, and G. Grübel, “Structure beyond pair correlations: X-ray cross- correlation from colloidal crystals,” J. Appl. Cryst. 49(Pt 6), 2046–2052 (2016). 14. M. A. Schroer, C. Gutt, and G. Grübel, “Characteristics of angular cross correlations studied by light scattering from two-dimensional microsphere films,” Phys. Rev. E Stat. Nonlin. Soft Matter Phys. 90(1), 012309 (2014). 15. T. Latychevskaia, G. F. Mancini, and F. Carbone, “The role of the coherence in the cross-correlation analysis of diffraction patterns from two-dimensional dense mono-disperse systems,” Sci. Rep. 5, 16573 (2015). 16. G. F. Mancini, T. Latychevskaia, F. Pennacchio, J. Reguera, F. Stellacci, and F. Carbone, “Order/Disorder Dynamics in a Dodecanethiol-Capped Gold Nanoparticles Supracrystal by Small-Angle Ultrafast Electron Diffraction,” Nano Lett. 16(4), 2705–2713 (2016). 17. J. Rajeswari, P. Huang, G. F. Mancini, Y. Murooka, T. Latychevskaia, D. McGrouther, M. Cantoni, E. Baldini, J. S. White, A. Magrez, T. Giamarchi, H. M. Rønnow, and F. Carbone, “Filming the formation and fluctuation of skyrmion domains by cryo-Lorentz transmission electron microscopy,” Proc. Natl. Acad. Sci. U.S.A. 112(46), 14212–14217 (2015). 18. A. Rundquist, C. G. Durfee 3rd, Z. Chang, C. Herne, S. Backus, M. M. Murnane, and H. C. Kapteyn, “Phase- Matched Generation of Coherent Soft X-rays,” Science 280(5368), 1412–1415 (1998). 19. R. A. Bartels, A. Paul, H. Green, H. C. Kapteyn, M. M. Murnane, S. Backus, I. P. Christov, Y. Liu, D. Attwood, and C. Jacobsen, “Generation of Spatially Coherent Light at Extreme Ultraviolet Wavelengths,” Science 297(5580), 376–378 (2002). 20. A. McPherson, G. Gibson, H. Jara, U. Johann, T. S. Luk, I. A. McIntyre, K. Boyer, and C. K. Rhodes, “Studies of multiphoton production of vacuum-ultraviolet radiation in the rare gases,” J. Opt. Soc. Am. B 4, 595 (1987). 21. P. B. Corkum, “Plasma Perspective on Strong Field Multiphoton Ionization,” Phys. Rev. Lett. 71(13), 1994– 1997 (1993). 22. X. Zhang, A. R. Libertun, A. Paul, E. Gagnon, S. Backus, I. P. Christov, M. M. Murnane, H. C. Kapteyn, R. A. Bartels, Y. Liu, and D. T. Attwood, “Highly coherent light at 13 nm generated by use of quasi-phase-matched high-harmonic generation,” Opt. Lett. 29(12), 1357–1359 (2004). 23. H. C. Kapteyn, M. M. Murnane, and I. P. Christov, “Extreme nonlinear optics: Coherent x-rays from lasers,” Phys. Today 58, 39–46 (2005). 24. F. Krausz and M. Ivanov, “Attosecond physics,” Rev. Mod. Phys. 81, 163–234 (2009). 25. Z. Tao, C. Chen, T. Szilvási, M. Keller, M. Mavrikakis, H. Kapteyn, and M. Murnane, “Direct time-domain observation of attosecond final-state lifetimes in photoemission from solids,” Science 353(6294), 62–67 (2016). 26. C. Chen, Z. Tao, A. Carr, P. Matyba, T. Szilvási, S. Emmerich, M. Piecuch, M. Keller, D. Zusin, S. Eich, M. Rollinger, W. You, S. Mathias, U. Thumm, M. Mavrikakis, M. Aeschlimann, P. M. Oppeneer, H. Kapteyn, and M. Murnane, “Distinguishing attosecond electron-electron scattering and screening in transition metals,” Proc. Natl. Acad. Sci. U.S.A. 114(27), E5300–E5307 (2017). 27. D. Sayre, “Some implications of a theorem due to Shannon,” Acta Crystallogr. 5, 843 (1952). 28. J. Miao, D. Sayre, and H. N. Chapman, “Phase retrieval from the magnitude of the Fourier transforms of Vol. 26, No. 9 | 30 Apr 2018 | OPTICS EXPRESS 11395 nonperiodic objects,” J. Opt. Soc. Am. A 15, 1662 (1998). 29. J. R. Fienup, “Reconstruction of an object from the modulus of its Fourier transform,” Opt. Lett. 3(1), 27–29 (1978). 30. J. Gulden, O. M. Yefanov, A. P. Mancuso, R. Dronyak, A. Singer, V. Bernátová, A. Burkhardt, O. Polozhentsev, A. Soldatov, M. Sprung, and I. A. Vartanyants, “Three-dimensional structure of a single colloidal crystal grain studied by coherent x-ray diffraction,” Opt.